FiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens


 Damon Willis
 1 years ago
 Views:
Transcription
1 Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: FiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens ABSTRACT: Experimental results showed that ASTM D 638 Type IV flat tension specimens, made of a Nylon11 matrix containing a large volume concentration of NdFeB particulates, failed at a location where the straight gage section of the specimen ends and the curved transition region begins. The stress distribution in this specimen was analyzed using the finiteelement method, and it was found that there is a stress concentration at this location. The stress distributions in tension specimens with both single and doublearc transition regions were analyzed and stress concentration factors were calculated. A linear relationship between the magnitude of the stress concentration factor and the ratio of the width in the gage section and the arc radius of the transition region is identified. This study shows that it is possible to reduce the magnitude of the stress concentration factor for the ASTM D 638 Type IV flat tension specimen by redesigning the specimen geometry without changing its overall size. KEYWORDS: stress concentration factor, finiteelement analysis, tensile strength Recent advancements in injection molding have made it a popular manufacturing method for costeffective, highvolume production of plastic and particlereinforced plastic composites. ASTM Standard D 638 [1], a standard test method for tensile strength of plastics, has been used widely in the industry to evaluate the tensile strength of plasticbased materials. In the absence of test methods for the tensile evaluation of particulatereinforced plastics, the ASTM D 638 test method also has been used to evaluate these reinforced plastic composites. Figure 1a shows a fractured ASTM D 638 Type IV specimen made of Nylon11 bonded NdFeB particles. This material, which contains 59.7 vol% of brittle NdFeB particles, is formulated for permanent magnet applications. The high percentage of NdFeB particles is necessary to achieve the desired magnetic properties for electrical motor and actuator applications. However, the high percentage of NdFeB particles also results in a material with reduced ductility [2 4]. The tensile evaluation of plasticbonded NdFeB magnets has shown that fracture almost always initiates at a location where the straight gage section of the specimen ends and the curved transition region begins. This location is marked as Point B in Fig. 1a. The failure at Point B, which is outside the uniformly loaded straight gage section, is due to a stress concentration and can lead to an underestimate of the tensile strength. Such stress concentration is not a problem for ductile materials because the large plastic deformation will redistribute the stress. For example, Fig. 1b shows a deformed ASTM D 638 Type IV tension specimen made of pure Nylon11. This specimen continued to deform extensively without fracturing at the location of initial stress concentration. Manuscript received 5/2/2002; accepted for publication 11/13/2002; published 11/18/ Department of Mechanical and Aerospace Engineering, North Carolina State University, Raleigh, NC Department of Mechanical Engineering, University of Michigan, Ann Arbor, MI High Temperature Materials Laboratory, Oak Ridge National Laboratory, Oak Ridge, TN Department of Materials Science and Engineering, North Carolina State University, Raleigh, NC As engineered and particlereinforced plastics become stronger and in some cases more brittle, the stress concentration in current tension specimen geometries has become an issue of concern. One of the objectives in this research is to analyze the stress concentration factor [5] on specimens specified in ASTM D 638 using the finiteelement method. Five types of specimens, designated as Type I, II, III, IV, and V, are defined in ASTM D 638. The shapes of Type III and V specimens are similar, which results in the same stress concentration factor at the location where the gage section ends and the transition region begins. Therefore, only Type I, II, III, and IV specimens were studied. In addition to these four standard tension specimens, the stress concentration factor for other specimen geometries with single or doublearc fillets was also analyzed using the finiteelement method to investigate possible ways to reduce the stress concentration without changing the overall size of specimens. The photoelastic method has been used in the past to study the stress concentration factors for shoulder fillets in flat plates [5 7]. Most of the cases studied have fillet radii much smaller than the width of the specimen. The shapes of tension specimens investigated in this research have the opposite trend: the fillet radii are much larger than the width of the specimen in order to reduce the stress concentration factor. For specimens with very small stress concentration factors, the finiteelement method with a reasonably fine mesh was applied to analyze the stress distributions and estimate the stress concentration factors. The finiteelement method has been applied previously to the design of flat tension specimens of advanced composites [8], ceramic matrix composites [9], and monolithic ceramics for creep testing [10]. Oplinger et al. [11] has studied the use of streamlined specimens to reduce the tensile and shear stress concentration in composite specimens. In this paper, first the finiteelement modeling of tension specimens is introduced. The stress concentration factor is defined. The distribution of von Mises stresses for four types of specimens specified in ASTM Standard D 638 is presented. The stress concentration factors of other specimen shapes with single and doublearc fillets are analyzed. Finally, a correlation between the magnitude of the stress concentration factor and the ratio of arc radius and width of the gage section is established. Copyright 2003 by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA
2 2 JOURNAL OF TESTING AND EVALUATION FiniteElement Modeling The twodimensional plane stress sixnode and twelve degreeoffreedom triangular linear elastic element was selected to model the flatplate tension specimens. The commercially available AN SYS finiteelement analysis software and its mesh generator were used. Figure 2 shows the finiteelement meshes used to model the four types of ASTM D 638 tension specimens. Due to the symmetry of the specimen geometry, only one quarter of the specimen is modeled. Point O is the center of the specimen. Lines OA and OE are the symmetry planes of the specimen. Point O is fixed in both the X and Ydirections. Nodes on Line OA have zero displacement in the Xdirection and are free to move in the Ydirection. Nodes on Line OE have zero displacement in the Ydirection and are free to move in the Xdirection. Nodes on Line ED are prescribed a uniform 0.1mm displacement in the Xdirection and zero displacement in the Ydirection. This is intended to simulate the holding of both ends in the wide section of the tension specimen using perfectly rigid grips. The extension of the specimen under this condition is 0.2 mm. In actual tensile tests, the specimen is clamped and pulled using a set of mechanical or hydraulic grips. The actual loading condition near the gripped area is therefore the combination of the normal compressive stress and inplane tensile and shear stresses. Dimensions of finiteelement meshes and the number of elements and nodes are summarized in the table in Fig. 2 for each type of ASTM D 638 specimen. OA is one half of the width of the gage FIG. 1 Pictures of ASTM D Type IV tension specimens: (a) Nylon11 bonded NdFeB (59.7 vol%) material tested with at 100 C, and (b) pure Nylon11 tested at 100 C. FIG. 3 Geometric model of the single and double radius transitional area. FIG. 2 Finiteelement mesh for four types of specimen in ASTM D
3 GARRELL ET AL. ON ASTM 638 TEST SPECIMENS 3 FIG. 4 Distribution of von Mises stress in ASTM D 638 tensile test specimens. (Value by the node represents the ratio of nodal von Mises stress relative to the maximum von Mises stress at node MX in Pa.) section, DE is one half of the width of the wide section, OE is one half of the length of the specimen, and AB is one half of the length of the gage section. Between Points B and C, the specimen changes from the narrow to the wide section. As shown in Figs. 2a, 2b, and 2c, Type I, II, and III specimens consist of a circular arc of radius r 1 between Points B and C. These are known as singlearc specimens. As shown in Fig. 2d, two radii, r 1 and r 2, are used to blend two arcs in the transitional region between Points B and C for the Type IV specimen. This is designated as the doublearc specimen. The geometrical relationships of the single and doublearc shape between Points B and C are shown in Fig. 3; w 1 and w 2 are widths of the narrow and wide section, respectively. As shown in Fig. 3a, the singleradius specimen has a continuous slope at Point B and a discontinuous slope at Point C. The doublearc specimen, as shown in Fig. 3b, has a continuous slope at all three transitional points: B, F, and C. Arcs BF and FC have the same angle, indicated by. The center of Arc BF, denoted as C 1 in Fig. 3a, has the same Xcoordinate as Point B. Similarly, the center of Arc CF, denoted as C 2, has the same Xcoordinate as Point C. These geometrical constraints together ensure a continuous slope at Points B, F, and C for the doublearc specimen. A hydrostatic stressdependent yield criterion is usually used to analyze stress concentrations in plastics [12,13]. The yield criterion for magnetic particle reinforced plastics has not yet been studied. The maximum von Mises stress was used to calculate the stress concentration factor and to identify the location that possibly initializes the fracture. In addition to the von Mises stress, the maximum principal stress, which is more suitable for the analysis of brittle materials, was also applied to calculate the stress concentration factor. The finiteelement analysis provided results of stress components and the von Mises and principal stress for each node. The nodal stress was used to calculate the stress concentration factor, K f. max K f (1) nominal where max is either the maximum nodal von Mises stress or maximum first principal stress, and nominal is either the average von Mises stress or the average first principal stress on nodes in the gage section. Finiteelement analysis results show that the variation of von Mises stress among nodes in the gage section is very small, less than 1.5%. An elastic modulus of 130 MPa and Poisson s ratio of 0.3 were used in the finiteelement analysis.
4 4 JOURNAL OF TESTING AND EVALUATION FiniteElement Analysis of Four Types of Tension Specimens Figure 4 shows the distribution of von Mises stress for ASTM D 638 Type I, II, III, and IV standard tension specimens. For each specimen, an overview and another enlarged view of the von Mises TABLE 1 The stress concentration for different single and doubleradius tension specimen geometry. Designation r 1 (mm) r 2 (mm) w 1 /r 1 K f ASTM Type I D 638 Type II Type III Type IV Single SI radius SII tension SIII specimen SIV SV SVI SVII Double DI radius DII* tension DIII specimen DIV DV DVI DVII * The same geometry as Type IV. stress distribution is presented. The enlarged view is centered about Point B to identify the increase in von Mises stress. In Fig. 4, MX and MN mark the nodes with maximum and minimum von Mises stress, respectively. As shown in the overview of the specimen, Node MN is close to Point C. In the enlarged view, the location of Node MX relative to Node B can be seen. Node MX is next to Node B, as in Type I and II, or a node away from Node B, as in Type III and IV. It is noted that the mesh shown in the enlarged view represents the exaggeratedly deformed finiteelement mesh from the ANSYS output. Node B, originally located at the intersection of a straight line and an arc, can be seen on a slightly curved region after deformation. The ratio of nodal von Mises stress relative to the maximum von Mises stress at Node MX is also presented in the enlarged view on nodes around Points B and MX in Fig. 4. For Type I, II, and III specimens, the overview of von Mises stress distribution does not show the stress concentration. Upon closely examining the distribution of von Mises stress around Point MX in the enlarged view, all four types of ASTM D 638 tension specimens demonstrate different levels of stress concentration at Node MX. The von Mises stress at Node MX ( max ) and at nodes in the gage section ( nominal ) were extracted from the finiteelement output and substituted into Eq 1 to calculate the stress concentration factor, K f. Results of K f are listed in Table 1. Type IV and II specimens have the highest and lowest K f, and 1.014, respectively. It was found that K f has an almost linear relationship versus the parameter w 1 /r 1, as shown in Fig. 5, for the four types of ASTM D 638 specimen. FIG. 5 The stress concentration factor versus ratio of gage section width and radius for five types of ASTM D 638 specimens and the single and doubleradius specimens.
5 GARRELL ET AL. ON ASTM 638 TEST SPECIMENS 5 Tension specimens with low w 1 /r 1 ratio usually have large arc radius and are longer than specimens with high w 1 /r 1. For example, as shown in Fig. 2 and Table 1, Type II and IV specimens have the same width in the gage section and different radius r 1. The Type II specimen has a larger arc radius, which makes the specimen longer and has lower w 1 /r 1 and K f. Longer and bigger tension specimens are unattractive because they require more material and a bigger die for injection molding and cost more to produce. Instead of using the von Mises stress, the maximum principal stress and nominal principal stress were extracted from the finiteelement output and substituted into Eq 1 to calculate K f. For all four types of specimens, the difference in K f based on von Mises and maximum principal stresses is very small, less than FiniteElement Analysis of Single and DoubleArc Tension Specimens In this section, the investigation of stress distribution in alternative tension specimen geometries that maintain the same overall size as the Type IV specimen is discussed. The objective is to identify the geometric parameters that would reduce the magnitude of K f. The width (w 1 ) and length of the gage section are 6 and 13 mm, respectively. The width of the wide section, w 2, is 19 mm. Two groups of sample geometry were studied. One group consists of singlearc specimens, similar to those in Type I, II, and III. Another group has the doublearc geometry, similar to the Type IV specimen. SingleArc Specimens As shown in Table 1, seven single radius curves are used to blend between Points B and C. The minimum radius of Arc BC is 6.5 mm ( (w 2 w 1 )/2). The specimens with radii of 6.5, 9, 13, 19, 28, 39, or 52 mm at Arc BC were designated as SI to SVII, respectively. The shape and finiteelement mesh of three selected specimens, SI, SIV, and SVII, are shown in Fig. 6. For specimens with arc radius equal to or less than 39 mm, the overall length of the original Type IV specimen can be maintained. The K f of the 39mm radius singlearc specimen (SVI), as shown in Table 1, is This is significantly lower than K f of of the Type IV specimen. Plots of K f versus w 1 /r 1 for these seven specimens are shown in Fig. 5. The larger radius of arc BC lowers both w 1 /r 1 and K f. Figure 5 also shows that the relationship between K f and w 1 /r 1 is almost linear and matches the trend of Type I to IV specimens. DoubleArc Specimens Seven doublearc specimens, denoted as DI to DVII, were studied as well. As shown in Fig. 3, the values of r 1 and r 2 in the doublearc geometry can be reversed and still maintain the continuity of both position and slope at Points B, F, and C. This special geometrical characteristic of the doublearc shape was used to define conjugate pairs of specimens. As shown in Table 1, DI (r 1 9 mm, r 2 30 mm) and DVII (r 1 30 mm, r 2 9 mm) form a conjugate pair of doublearc specimens. DII (r 1 14 mm, r 2 25 mm) and DVI (r 1 25 mm, r 2 14 mm) as well as DIII (r 1 17 mm, r 2 22 mm) and DV (r 1 22 mm, r 2 17 mm) are another two sets of conjugate doublearc specimens. It is noted that the DII specimen has the same geometry as the ASTM D 638 Type IV specimen. The intent is to investigate the change in K ƒ of a conjugate doublearc specimen. The DIII specimen has the same r 1 and r 2, both equal to 19.5 mm. The shape and finiteelement mesh of three selected specimens, DI, DIV, and DVII, are shown in Fig. 6. Finiteelement analysis results of K f versus w 1 /r 1 for seven doublearc specimens are listed in Table 1 and plotted in Fig. 5. It is important to note that the value of r 2 does not affect K f. By just switching the two arcs of the original Type IV specimen, the K f was reduced from to By further increasing r 1 to 30 mm without changing the overall size of the Type IV specimen, K f was reduced to Modeling of the Stress Concentration Factor As shown in Fig. 5, a straight line can be used to determine K f for various w 1 /r 1. Linear regression analysis was performed on all 17 data points, including the four types of specimen specified by ASTM D 638 and the seven singlearc and six doublearc specimens. The following model is obtained: K f (w 1 /r 1 ) (2) Equation 2 can be used to predict the K f based on w 1 /r 1 and may be useful for new tension specimen design. FIG. 6 Finiteelement meshes for selected single and doublearc specimens (3 mm halfwidth in the gage section for all specimens).
6 6 JOURNAL OF TESTING AND EVALUATION The linear trend indicates the possibility that an analytical solution for the stress distribution in this geometrical configuration may exist. This requires further investigation. Concluding Remarks The stress distribution of four types of tension specimens recommended in ASTM D 638 was investigated through the use of the finiteelement technique. It was found that the location of maximum von Mises stress for Type IV geometry coincided with the location of experimentally observed failures in brittle specimens made of Nylon11 bonded NdFeB particles. This study identified a solution to reduce the magnitude of stress concentration by increasing the radius of the arc in the transitional area. A linear correlation of stress concentration factor K f versus w 1 /r 1 was identified and a linear model was established to predict the K f based on w 1 /r 1. Results obtained in this research can help establish standards and aid in the design of specimen geometry for tension testing of brittle particlereinforced composites. Acknowledgments A portion of this research was sponsored by the User program of the High Temperature Material Laboratory of Oak Ridge National Laboratory and by National Science Foundation Grant (Dr. K. P. Rajurkar, Program Director). References [1] ASTM D : Standard Test Method for Tensile Strength of Plastics, Annual Book of ASTM Standards, ASTM International, West Conshohocken, PA, [2] Garrell, M. G., Ma, B. M., LaraCurzio, E., Shih, A. J., and Scattergood, R. O., Mechanical Properties of Nylon Bonded NdFeB Permanent Magnets, Journal of Magnetism and Magnetic Materials, accepted for publication. [3] Garrell, M. G., Ma, B. M., LaraCurzio, E., Shih, A. J., and Scattergood, R. O., Mechanical Properties of PolyphenyleneSulfide (PPS) Bonded NdFeB Permanent Magnets, Materials Science and Engineering: A, submitted. [4] Garrell, M. G., Mechanical Properties of Injection Molded Permanent Magnets, M.S. thesis, North Carolina State University, Raleigh, NC, April [5] Pilkey, W. D., Peterson s Stress Concentration Factors, 2nd ed., John Wiley & Sons, New York, [6] Wilson, L. H. and White, D. J. StressConcentration Factors for Shoulder Fillets and Grooves in Plates, Journal of Strain Analysis, Vol. 8, 1973, pp [7] Frocht, M. M. Factor of Stress Concentration Photoelastically Determined, Transactions of ASME, 1935, Vol. 57, pp. A67 A68. [8] Worthem, D. W., Flat Tension Specimen Design for Advanced Composites, NASA Technical Report CR , NASA Lewis Research Center, Cleveland, OH, [9] Shi, J., Brady, L., and Ireson, A., Design of Room Temperature Tension Specimen Made of Ceramic Matrix Composites, Key Engineering Materials, Vol , Trans Tech Publications, 1999, pp [10] Wang, Z, Chiang, C. K., and Chuang, T.J., Optimum Design of a Ceramic Tensile Creep Specimen Using a Finite Element Method, Journal of Research of the National Institute of Standards and Technology, Vol. 102, 1997, pp [11] Oplinger, D. W., Parker, B. S., Gandhi, K. R., Lamothe, R., and Foley, G., On the Streamline Specimen for Tension Testing of Composite Materials, Recent Advances in Composites in the United States and Japan, ASTM STP 864, J. R. Vinson and M. Taya, Eds., ASTM International, West Conshohocken, PA, 1985, pp [12] McCrum, N. G., Buckley, C. P., and Bucknall, C. B., Principles of Polymer Engineering, 2nd ed., Oxford University Press, Oxford, [13] Courtney, T. H., Mechanical Behavior of Materials, 2nd ed., McGrawHill, New York, 2000.
Structural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More information5. STRESS CONCENTRATIONS. and strains in shafts apply only to solid and hollow circular shafts while they are in the
5. STRESS CONCENTRATIONS So far in this thesis, most of the formulas we have seen to calculate the stresses and strains in shafts apply only to solid and hollow circular shafts while they are in the elastic
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationBurst pressure estimation of reworked nozzle weld on spherical domes
Indian Journal of Engineering & Materials Science Vol. 21, February 2014, pp. 8892 Burst pressure estimation of reworked nozzle weld on spherical domes G Jegan Lal a, Jayesh P a & K Thyagarajan b a Cryo
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationSIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS
43rd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Con 2225 April 2002, Denver, Colorado SIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS Erik C. Mellquistand Anthony M.
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationNonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield Surface
Transaction A: Civil Engineering Vol. 16, No. 6, pp. 512{519 c Sharif University of Technology, December 2009 Research Note Nonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationStresses Analysis of Petroleum Pipe Finite Element under Internal Pressure
ISSN : 4896, Vol. 6, Issue 8, ( Part 4 August 06, pp.338 RESEARCH ARTICLE Stresses Analysis of Petroleum Pipe Finite Element under Internal Pressure Dr.Ragbe.M.Abdusslam Eng. Khaled.S.Bagar ABSTRACT
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationMECHANICS OF MATERIALS
2009 The McGrawHill Companies, Inc. All rights reserved. Fifth SI Edition CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes:
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationME 354, MECHANICS OF MATERIALS LABORATORY COMPRESSION AND BUCKLING
ME 354, MECHANICS OF MATERIALS LABATY COMPRESSION AND BUCKLING PURPOSE 01 January 2000 / mgj The purpose of this exercise is to study the effects of end conditions, column length, and material properties
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationStandard Practice for Heat Aging of Plastics Without Load 1
Designation: D 3045 92 (Reapproved 2003) Standard Practice for Heat Aging of Plastics Without Load 1 This standard is issued under the fixed designation D 3045; the number immediately following the designation
More informationPlasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur
Plasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 9 Table of Contents 1. Plasticity:... 3 1.1 Plastic Deformation,
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationStandard Test Methods for GlassBonded Mica Used as Electrical Insulation 1
Designation: D 1039 94 (Reapproved 1999) e1 An American National Standard Standard Test Methods for GlassBonded Mica Used as Electrical Insulation 1 This standard is issued under the fixed designation
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationTABLE OF CONTENTS CHAPTER TITLE PAGE DECLARATION DEDICATION ACKNOWLEDGEMENT ABSTRACT ABSTRAK
vii TABLE OF CONTENTS CHAPTER TITLE PAGE DECLARATION DEDICATION ACKNOWLEDGEMENT ABSTRACT ABSTRAK TABLE OF CONTENTS LIST OF TABLES LIST OF FIGURES LIST OF ABBREVIATIONS LIST OF SYMBOLS ii iii iv v vi vii
More informationFinite element simulations of fretting contact systems
Computer Methods and Experimental Measurements for Surface Effects and Contact Mechanics VII 45 Finite element simulations of fretting contact systems G. Shi, D. Backman & N. Bellinger Structures and Materials
More information9 MECHANICAL PROPERTIES OF SOLIDS
9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body
More informationModelling the behaviour of plastics for design under impact
Modelling the behaviour of plastics for design under impact G. Dean and L. Crocker MPP IAG Meeting 6 October 24 Land Rover door trim Loading stages and selected regions Project MPP7.9 Main tasks Tests
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationSolid Mechanics Chapter 1: Tension, Compression and Shear
Solid Mechanics Chapter 1: Tension, Compression and Shear Dr. Imran Latif Department of Civil and Environmental Engineering College of Engineering University of Nizwa (UoN) 1 Why do we study Mechanics
More informationFE Modeling of HSECTION Connecting Rod
FE Modeling of HSECTION Connecting Rod Virendra Kumar Verma,Shailendra Kumar, Ashish Gupta P.G Student, Department of Mechanical Engineering, Babu Banarasi Das University, Lucknow, India P.G Student,
More information7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment
7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that
More informationA Finite Element Study of ElasticPlastic Hemispherical Contact Behavior against a Rigid Flat under Varying Modulus of Elasticity and Sphere Radius
Engineering, 2010, 2, 205211 doi:10.4236/eng.2010.24030 Published Online April 2010 (http://www. SciRP.org/journal/eng) 205 A Finite Element Study of ElasticPlastic Hemispherical Contact Behavior against
More informationChapter 6: Plastic Theory
OHP Mechanical Properties of Materials Chapter 6: Plastic Theory Prof. Wenjea J. Tseng 曾文甲 Department of Materials Engineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W. F.
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationLife Prediction Under Multiaxial Fatigue
Lie Prediction Under Multiaxial Fatigue D. Ramesh and M.M. Mayuram Department o Mechanical Engineering Indian Institute o Technology, Madras Chennai600 036 (India) email: mayuram@iitm.ac.in ABSTRACT
More informationEffect Of The InSitu Stress Field On Casing Failure *
Effect Of The InSitu Stress Field On Casing Failure * Tang Bo Southwest Petroleum Institute, People's Republic of China Lian Zhanghua Southwest Petroleum Institute, People's Republic of China Abstract
More informationVolume 2 Fatigue Theory Reference Manual
Volume Fatigue Theory Reference Manual Contents 1 Introduction to fatigue 1.1 Introduction... 11 1. Description of the applied loading... 11.3 Endurance curves... 13 1.4 Generalising fatigue data...
More informationREPORT TO DFLEX LTD APRIL 2009 REPORT. (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009)
REPORT (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009) Finite Element Modelling of Rigidity of Fishing Rods with Various Crosssections Report to DFlex Ltd by Z Guan Department of Engineering,
More informationSIMPLIFIED CONCRETE MODELING WITH *MAT_CONCRET_DAMAGE_REL3
SIMPLIFIED CONCRETE MODELING WITH *MAT_CONCRET_DAMAGE_REL3 Leonard E Schwer Schwer Engineering & Consulting Services, Windsor CA, USA and L. Javier Malvar Karagozian & Case Structural Engineers, Burbank
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationLecture #2: Split Hopkinson Bar Systems
Lecture #2: Split Hopkinson Bar Systems by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing 2015 1 1 1 Uniaxial Compression
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationMAE 322 Machine Design Lecture 2. Dr. Hodge Jenkins Mercer University
MAE 322 Machine Design Lecture 2 Dr. Hodge Jenkins Mercer University Statics Load Failure Theories to Understand Maximum Normal Stress (MNS) Maximum Shear Stress (MSS) Distortion Energy (DE) CoulombMohr
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationALGORITHM FOR NONPROPORTIONAL LOADING IN SEQUENTIALLY LINEAR ANALYSIS
9th International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS9 Chenjie Yu, P.C.J. Hoogenboom and J.G. Rots DOI 10.21012/FC9.288 ALGORITHM FOR NONPROPORTIONAL LOADING
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationWhen you are standing on a flat surface, what is the normal stress you exert on the ground? What is the shear stress?
When you are standing on a flat surface, what is the normal stress you exert on the ground? What is the shear stress? How could you exert a nonzero shear stress on the ground? Hydrostatic Pressure (fluids)
More informationStudy of Circular and Elliptical Holes as a Stress Relieving Feature in Spur Gear
Study of Circular and Elliptical Holes as a Stress Relieving Feature in Spur Gear Prof. S.B.Naik 1, Mr. Sujit R. Gavhane 2 Asst. Prof. Department of Mechanical Engineering, Walchand Institute of Technology,
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationEFFECT OF STRAIN HARDENING ON ELASTICPLASTIC CONTACT BEHAVIOUR OF A SPHERE AGAINST A RIGID FLAT A FINITE ELEMENT STUDY
Proceedings of the International Conference on Mechanical Engineering 2009 (ICME2009) 2628 December 2009, Dhaka, Bangladesh ICME09 EFFECT OF STRAIN HARDENING ON ELASTICPLASTIC CONTACT BEHAVIOUR OF A
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationDEVELOPMENT OF TEST GUIDANCE FOR COMPACT TENSION FRACTURE TOUGHNESS SPECIMENS CONTAINING NOTCHES INSTEAD OF FATIGUE PRECRACKS
Transactions, SMiRT23 Division II, Paper ID 287 Fracture Mechanics and Structural Integrity DEVELOPMENT OF TEST GUIDANCE FOR COMPACT TENSION FRACTURE TOUGHNESS SPECIMENS CONTAINING NOTCHES INSTEAD OF
More informationA FINITE ELEMENT STUDY OF ELASTICPLASTIC HEMISPHERICAL CONTACT BEHAVIOR AGAINST A RIGID FLAT UNDER VARYING MODULUS OF ELASTICITY AND SPHERE RADIUS
Proceedings of the International Conference on Mechanical Engineering 2009 (ICME2009) 2628 December 2009, Dhaka, Bangladesh ICME09 A FINITE ELEMENT STUDY OF ELASTICPLASTIC HEMISPHERICAL CONTACT BEHAVIOR
More informationMechanical behaviour of wood in the orthotropic directions
Mechanical behaviour of wood in the orthotropic directions J.. Morais 1, J. C. Xavier 1, N. M. Dourado 1, J.. ousada 2 1 Departamento de Engenharias, ICETA/UTAD, Portugal 2 Departamento de Florestal, ICETA/UTAD,
More informationEffective stress assessment at rectangular rounded lateral notches
Focussed on characterization of crack tip fields Effective stress assessment at rectangular rounded lateral notches Enrico Maggiolini, Roberto Tovo, Paolo Livieri University of Ferrara Enrico.maggiolini@unife.it,
More informationLINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL
LINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL SREELATHA P.R * M.Tech. Student, Computer Aided Structural Engineering, M A College of Engineering, Kothamangalam 686 666,
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationFinite Element Analysis of Bicycle Crank
IJSTE  International Journal of Science Technology & Engineering Volume 3 Issue 10 April 2017 ISSN (online): 2349784X Finite Element Analysis of Bicycle Crank Mohammed Asif Kattimani Assistant Professor
More informationThe plastic behaviour of silicon subjected to microindentation
JOURNAL OF MATERIALS SCIENCE 31 (1996) 56715676 The plastic behaviour of silicon subjected to microindentation L. ZHANG, M. MAHDI Centre for Advanced Materials Technology, Department of Mechanical and
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationFinite Element Analysis of Compression of Thin, High Modulus, Cylindrical Shells with LowModulus Core
Finite Element Analysis of Compression of Thin, High Modulus, Cylindrical Shells with LowModulus Core Robert S. Joseph Design Engineering Analysis Corporation, McMurray, PA ABSTRACT Long, cylindrical
More informationTolerance Ring Improvement for Reducing Metal Scratch
International Journal of Scientific and Research Publications, Volume 2, Issue 11, November 2012 1 Tolerance Ring Improvement for Reducing Metal Scratch Pattaraweerin Woraratsoontorn*, Pitikhate Sooraksa**
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationFinal Design Project: Biodiesel Settling Tank Analysis
MESSIAH COLLEGE ENGR 495 Finite Element Methods Tuesday, December 16, 2003 : Biodiesel Settling Tank Analysis Brandon Apple Jon Bitterman Becky Gast Kyle McNamara ENGR 495 Finite Element Methods 1 Abstract
More informationLecture #8: Ductile Fracture (Theory & Experiments)
Lecture #8: Ductile Fracture (Theory & Experiments) by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing 2015 1 1 1 Ductile
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationStrength of Materials (15CV 32)
Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, StressStrain
More informationMECHANICS OF MATERIALS
Third CHTR Stress MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University and Strain xial oading Contents Stress & Strain: xial oading Normal
More informationExcerpt from the Proceedings of the COMSOL Conference 2010 Boston
Excerpt from the Proceedings of the COMSOL Conference 21 Boston Uncertainty Analysis, Verification and Validation of a Stress Concentration in a Cantilever Beam S. Kargar *, D.M. Bardot. University of
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationFatigue Algorithm Input
Methods Fatigue Algorithm Input By default, fesafe analyses stress datasets that contain elastic stresses The calculation of elasticplastic stressstrains, where necessary, is performed in fesafe using
More informationLecture #7: Basic Notions of Fracture Mechanics Ductile Fracture
Lecture #7: Basic Notions of Fracture Mechanics Ductile Fracture by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing
More informationINFLUENCE OF THE LOCATION AND CRACK ANGLE ON THE MAGNITUDE OF STRESS INTENSITY FACTORS MODE I AND II UNDER UNIAXIAL TENSION STRESSES
INFLUENCE OF THE LOCATION AND CRACK ANGLE ON THE MAGNITUDE OF STRESS INTENSITY FACTORS MODE I AND II UNDER UNIAXIAL TENSION STRESSES Najah Rustum Mohsin Southern Technical University, Technical InstituteNasiriya,
More information6 Examples of pneumatic structures and material models for membranes
6 Examples of pneumatic structures and material models for membranes This chapter is divided in two main topics: material models for membranes and static analysis of pneumatic structures. Initially uniaxial
More informationTOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS. Ford Research Laboratory, Ford Motor Company, Dearborn, MI 48121, U.S.A. 1.
TOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS M. D. Thouless, M. S. Kafkalidis, S. M. Ward and Y. Bankowski Department of Mechanical Engineering and Applied Mechanics, University of Michigan, Ann
More information